# Lab Report: Charpy Vee Notch

Good Essays
656 Words
Grammar
Plagiarism
Writing
Score
Lab Report: Charpy Vee Notch
Introduction:
The objective of the lab was to determine the amount of energy absorbed by a material during fracture. Another goal of this lab was to learn how to use impact-testing equipment and procedures. The lab materials included a specimen, which consists of a bar of either 6061-T6 Aluminum or 2024 Aluminum having a notch that was machined and an apparatus made up of a pendulum to impact the notched specimen.
Procedure:
The apparatus’ dimensions and the mass of the pendulum were measured and recorded. The angles of the pendulum were recorded at the loaded and rest position. The specimen was then placed onto the apparatus with the notch side aligned so the pendulum will hit there. The apparatus’ pendulum was dropped from a known height
Generally, the 6061-T6 specimens absorbed 34.14 (ft-lb) more energy than the 2024 specimens. This means that the 6061-T6 specimens are tougher than then the 2024 specimens because they can absorb more energy before fracturing. From the table it is clear that with the smaller degrees. Figure 1: Charpy Vee Notch Energy Graph …show more content…
The probability plot shows that the AA6061 clearly has a higher flexure strength than AA2024. In addition, the data points on the graph are relatively linear suggesting there wasn’t any real outliers in the data. This is also suggested by the relativity low standard deviation shown are the right side of the graph.

Examination of the specimens: The 6061-T6 specimens experienced a deformation just enough to pass. The 6061-T6 specimens did not completely break apart as shown in Figure 2. In addition, the 6061-T6 specimens ended up with a rough surface as shown in Figure 3. Also, there were some contractions in the Z direction as shown in 2 and Figure 3. Since the 6061-T6 specimens deformed without completely fracturing apart this aligns with the result section stating that it is tougher and can absorb more energy. On the other hand, the 2024 specimens completely broke into two as shown in Figure 2. The 2024 specimens had a relatively smooth surface as shown in Figure 3. Moreover, the 2024 specimens had no contraction in the Z direction as shown in Figure 2 and Figure 3. Since the 2024 specimens completely fractured apart into two unlike the 6061-T6 specimens shows that it is less tough and can’t absorb as much energy.

Figure 2: 2024 Specimen (Left) and 6061-T6 Specimen (Right) Fracture

## You May Also Find These Documents Helpful

• Good Essays

3. brittleness. 1. II and III only 4. density. 2. All of these 3.…

• 1541 Words
• 14 Pages
Good Essays
• Good Essays

This lab was performed to fully comprehend the temperature dependency of the fracture toughness of the Aluminum and Steel. It was also executed to discover the ductile-brittle transition of each.…

• 521 Words
• 3 Pages
Good Essays
• Better Essays

* Simple fracture. This is when your injury causes a single crack across the bone.…

• 3984 Words
• 16 Pages
Better Essays
• Powerful Essays

The experiment observed the mechanical deformation process of different materials by three tests: tensile test, impact test, and fracture-toughness test. The materials evaluated in the tensile test were annealed 1045 steel, cold rolled 1045 steel, 2024-T4 aluminum and cast iron. 2024-T4 aluminum is concluded to be most ductile (25.7 % reduction in area) and cast iron the most brittle (123 MPa). Effects of cold rolling in 1045 steel are apparent, as it has the highest strength among the materials tested (402 MPa yield strength). Impact test measured the impact energy of 1045 steel, 2024 aluminum, polypropylene (PP), and poly(methyl methacrylate) (PMMA). This test also observed the effect of temperature on material ductility. The fracture-toughness test was performed on 2024-T4 aluminum to determine a KIC of 35.3 MPam. From the experiment, it was found that the brittle-ductile transition temperature of PP is between 0 0C and room temperature, whereas the transition temperature of 1045 steel is between 25 0C and 100 0C.…

• 3265 Words
• 14 Pages
Powerful Essays
• Powerful Essays

Experiment Two: Stiffness Report from laboratory work performed on 12 May 2011 as a part of the unit of study CIVL2201 Structural Mechanics…

• 2020 Words
• 9 Pages
Powerful Essays
• Better Essays

Out of the three materials tested, the steel 1045 exhibited the most elastic properties, with it being able to deform elastically for a greater amount of stress than for the other specimens, as indicated by its stress-strain curve as shown in figure 1, and further supported by it having the highest modulus of elasticity of all three specimens, as shown in table 2. The mild steel specimen had the second greatest modulus of elasticity, and the aluminium specimen had the lowest modulus of…

• 1478 Words
• 6 Pages
Better Essays
• Better Essays

Bibliography: Dowling NE (2007) Mechanical Behaviour of Materials 3 Ed. Pearson Prentice-Hall: New Jersey. Breburge B (1999) Cracks and Fracture. Academic Press: California. Gross D and Seeling T (2006) Fracture Mechanics with an Introduction to Micromechanics. Springer: Berlin. th Callister WD (2007) Materials Science and Engineering 7 ed. John Wiley and Sons, Inc: York.…

• 1581 Words
• 7 Pages
Better Essays
• Good Essays

Asbestos gave the break lining greater stability at higher temperatures, thus the linings are more resistant to break failure form the heat.…

• 553 Words
• 3 Pages
Good Essays
• Satisfactory Essays

Seeley, Fred B. , and Smith, James 0., Advanced Mechanics of Materials, Second Edition, John Wiley and Sons, Inc. , 1952.…

• 102672 Words
• 1663 Pages
Satisfactory Essays
• Satisfactory Essays

Engineering Fracture Mechanics Vol. 54, No. 2, pp. 263-300, 1996 Copyright © 1996 Elsevier Science Ltd. 0013-7944(95)00178-6 Printed in Great Britain. All rights reserved 0013-7944/96 \$15.00+ 0.00…

• 30030 Words
• 121 Pages
Satisfactory Essays
• Satisfactory Essays

The wound is less than 1cm long. It is usually a moderately clean puncture, through which a spike of bone has pierced the skin. There is little soft-tissue damage and no sign of crushing injury. The fracture is usually simple, transverse, or short oblique, with little comminution.…

• 339 Words
• 2 Pages
Satisfactory Essays
• Good Essays

information, what would be the stress needed to break the specimen of this material in a…

• 431 Words
• 2 Pages
Good Essays
• Good Essays

9. It is clear that the microhardness number increases with increasing load. It is evident from the above plot that the microhardness number of the crystal increases with increase in load which is in agreement with the reverse indentation size effect (ISE) [15] and also decreases with increase in temperature. The decrease in the value of hardness number with respect to increase in temperature can be attributed to the fact that, when the temperature increases, the average inter atomic distance becomes greater than that at room temperature due to lattice vibration. This leads to more and more lattice phonon interactions which causes the breaking of bond as well reduce the hardness value [16]. The maximum value of hardness number observed for 2PPA, crystal is 39.9 kg/mm2 at 50 g (room temperature) respectively. The load above these values develops multiple cracks on the crystal surface due to the release of internal stresses generated locally by…

• 719 Words
• 3 Pages
Good Essays
• Better Essays

The specimens that are used in this test are normalized in accordance with the standards. The purpose of this experiment is to analyse the hardenability of the three materials such as EN-3 (1015), EN-8 (1040) and EN-24 (4340).…

• 928 Words
• 4 Pages
Better Essays
• Good Essays

Fig. 4 shows that specimens subjected to minor axis bending failed at considerably lower load than those subjected to major axis bending. Rate of reduction of ultimate load is more pronounced in the case of minor axis bending. For example, the rate of reduction of ultimate load for S500 specimen, when e/xo increases from 0 to 2.8, is 5.7% and 56% for the specimen subjected to major axis bending and minor axis bending respectively. The corresponding rate of reduction of strength for S1100 specimens are 6.15% and 23.8% respectively. At larger eccentricity ratios (from 1.4 to 2.1), the curves become flatter…

• 865 Words
• 4 Pages
Good Essays